Summary of industrial failures caused by multiple crack interaction
This chapter aims to introduce the concept of fracture mechanics and numerical approaches to solve interacting cracks problems in solid bodies which involves elastic crack interaction. The elastic crack interaction is a result of changes in stress field distribution as the applied force is given during remote loading. The main emphasis is to address the computational evaluation on mechanistic models based on crack tip displacement, stress fields and energy flows for multiple cracks. This chapter start with a brief discussion on fracture and failure that promoted by interacting cracks from industrial cases to bring the issues of how important the crack interaction behaviour is. The present fracture and failure mechanism is assumed to exhibit the brittle fracture. Thus, the concept of linear elastic fracture mechanics (LEFM) is discussed regarding the crack interaction model formulation. As the elastic crack interaction is concerned, the previous analytical and numerical solution of crack interaction are elaborated comprehensively corresponds to fitness-for-service (FFS) as published by ASME boiler and pressure vessel code (Section XI, Articles IWA-3330), JSME fitness-for-service code and BSI PD6493 and BS7910. A new computational fracture mechanics algorithm is developed by adopting stress singularity approach in finite element (FE) formulation. The result of developed approach is discussed based on the crack interaction limit (CIL) aspects and crack unification limit (CUL) in pertinent to the equality of two cracks to single crack rules in FFS. As a conclusion, the FE formulated approach was found to be at agreeable accuracy with analytical formulation and FFS at certain range of crack interval.
2. Fracture and failures by interacting cracks
This section provides the overview of failure cases in industries and related fitness-for-sevice (FFS) codes which used to assess any cracks or flaws that detected in structures. The works on solution models for FFS codes improvement in specific cases of interacting cracks also discussed.
2.1. Industrial failures
In this section, the fracture and failure by interacting cracks is explained by examples from industrial failures. Mechanical structures and components are designed with multiple stress concentration features (SCF) such as notches, holes, corners and bends. For example, welding and riveting in joining and fastening process have consumed to the increase of stress concentration factor. In every SCF, there is a critical point that experienced the highest concentrated stress field, named as multiple stress riser points (MRSP). Under multiple mode of loading and environmental effect, the interaction between SCF and MRSP tends to form multiple cracks in various types of cracks (e.g. straight crack, surface crack and curved crack) before the cracks propagate in various path to coalescence, overlapping, overlapping, branching and finally fracture in brittle manner.
Crack interaction that induced from MRSP has caused many catastrophic failures, for example in aircraft fuselage (Hu, Liu, & Barter, 2009), F-18 Hornet bulkhead (Andersson et al., 2009), rotor fault (Sekhtar, 2008), gigantic storage tanks (Chang & Lin, 2006), oil tankers (Garwood, 2001), polypropylene tank (Lewis & Weidmann, 2001) and the most recent is the fail of helicopter longerons (J. A. Newman, Baughman, & Wallace, 2010). The recent lab experimental work on multiple crack initiation, propagation and coalescence by (Park & Bobet, 2010) and metallurgical work by (J. A. Newman et al., 2010) supported the important role of crack interaction in fracture and failure. The above cases proved how crucial and important the research on crack interaction is.
To explain further, failure in aircraft is considered as an example. Al Alloy has been extensively used for the fabrication of fuselage, wing, empennage, supporting structures that involve many fastening and joining points. Under static, cyclic loading and environmental effect, the micro-cracks are initiated from MRSP. To certain extent, out of many factors, brittle failure may happen through catastrophic failure (Hu, Liu, & Barter, 2009). As the distance between MRSP is close, the interaction between cracks is become more critical. The fracture behavior due to interacting cracks as the distance between cracks is closed need more understanding. The conventional fracture mechanics may be insufficient to support.
In this case, the advancement of computational fracture mechanic may contribute a lot in crack interaction research and increase the accuracy of failure prediction (Andersson et al., 2009). Most recent structural failure being reported is dealing with fuselage joints in large aircraft structures (Hu et al., 2009). The aircraft fuselage structure is made by 7050-T7451 aluminum alloy and designed to have multiple shallow notches that purposely used for lap joints. Due to environmental reaction and variable magnitude of operational loading, multi-site cracks are formed at MRSP. Therefore, the interaction of multi-site cracks is needed to be quantified for possible coalescence between cracks. The challenge is how to predict the accurate coalescence and fatigue crack growth for the multiple crack problems. Table 1 provides the list of industrial failures that originated from various kinds of multiple cracks. Under loading condition such as mechanical or thermal loading, it is observed that most of the cracks or flaws formation is start on the surface of the body rather than embedded inside the body.
|Multiple Cracks||Industrial Failures||References|
|Collinear cracks||Failure of crack arresters- stiffeners in aircraft structures||(Isida, 1973)|
|Parallel and layered cracks||Failure of welded-bonded structures in composite structures for aircraft||(Ratwani & Gupta, 1974)|
|Collinear cracks and edge cracks||Catastrophic fracture accidents of turbine or generator motor||(Matake & Imai, 1977; Pant, Singh, & Mishra, 2011; Sekhtar, 2008)|
|Elliptical cracks||Failure in boilers||(O'donoghue, Nishioka, & Atluri, 1984)|
|Collinear and radial cracks||Failure of pressurized thick-walled cylinder||(Chen & Liu, 1988; Kirkhope, Bell, & Kirkhope, 1991)|
|Collinear and micro-cracks||Failure of ceramic material in heat exchangers and automobiles||(Lam & Phua, 1991)|
|Parallel cracks||Failure of aero-engine turbine engines coatings||(Meizoso, Esnaola, & Perez, 1995)|
|Parallel edge cracks||Failure of actuator piston rods||(Rutti & Wentzel, 1997)|
|Edge cracks||Brittle failure of Oil Tanker structures at welded joints||(Garwood, 2001)|
|Array of edge cracks||Failure of heat-checked gun tubes and rapidly cooled pressure vessels||(Parker, 1999)|
|Semi-elliptical surface cracks||Failure in pressure vessel and piping components||(Moussa, Bell, & Tan, 1999; Murakami & Nasser, 1982)|
|Collinear cracks and flat elliptical cracks||Multiple site damage in aircraft structures||(Gorbatikh & Kachanov, 2000; Jeong & Brewer, 1995; Jones, Peng, & Pitt, 2002; Milwater, 2010; Pitt, Jones, & Atluri, 1999)|
|Multiple flaws and surface cracks||Failure of nuclear power plant components||(Kamaya, Miyokawa, & Kikuchi, 2010; Kobayashi & Kashima, 2000)|
|Penny-shaped cracks||Brittle fracture of welded structures in pressure vessels||(Saha & Ganguly, 2005)|
|Offset collinear and layered cracks||Fracture and catastrophic failure in polymeric structures||(Lewis & Weidmann, 2001; Sankar & Lesser, 2006; Weidmann & Lewis, 2001)|
|Interface cracks||Failure in electronic packages and micro-electro-mechanical systems (MEMS)||(Ikeda, Nagai, Yamanaga, & Miyazaki, 2006)|
|Parallel cracks||Fracture in functional gradient materials (FGM)||(Yang, 2009)|
|Short cracks and micro-cracks||Fracture in bones||(Lakes, Nakamura, Behiri, & Bonfield, 1990; Mischinski & Mural, 2011; Ural, Zioupos, Buchanan, & Vashishth, 2011)|
Crack interaction intensity exist in the form of stress shielding and amplification. The failure mechanism by cracks interaction may occurs under brittle, plastic and creep failure. In general, the interacting cracks problems that promotes the fracture and failure of structures are solved using the advancement of fracture mechanics. The fracture mechanics solution can be accomplished through analytical, numerical and experimental work. Based on the above individual approach or combination of them, typically the solution is represented by a model. The model may be defined based on the uncertainty input for the model such as crack geometry, loading and material properties. For crack interaction problems that randomness is relatively small, the deterministic analysis is the best to considered rather than probabilistic analysis. The model is suitable for any deterministic system response. However, when the randomness is relatively high, the model system response required a more robust solution, known as probabilistic approach.
Multiple cracks interaction can be defined into elastic crack interaction and plastic crack interaction that may be referred to theory of elasticity and plasticity, respectively. Under loading condition, the high stresses near crack tips usually accompanied by inelastic deformation and other non-linear effect. If the inelastic deformation and other non-linear effect are relatively small compared to crack sizes and other geometrical body characteristic, the linear theory is most adequate to address the crack interaction behavioral problems. Thus, the role of elastic driving force originated from crack tips can be translated into elastic crack interaction. Then, for every type of interaction, it may classified into interaction without crack propagation (EIWO) where the interaction occurs in the region of SIF and interaction with crack propagation (EIWI) occurs in the region of SIF . In this case of EIWO, the quantification of crack extension is neglected. The EIWO becomes the main issue of interaction in present study since it is inadequate investigation on crack interaction limit and multiple to single crack equivalencies. The study on EIWO is typically measured the fracture parameter and its behavior based on SIF while EIWI more focused to evaluation and prediction of crack path, propagation, coalescence, branching and crack arrestment. Under mechanical or thermal loading condition, the generated interaction will varies depends on type of loading mode (e.g. Mode I and Mode II) being applied. The preceding sections outlined the related fitness-for-service (FFS) codes in pertinent to failures that caused by crack interaction.
2.2. Fitness-for-Service (FFS) codes
This section presents the guidelinea that have been published in fitness-for-service (FFS) codes. The related investigation works also discussed as the FFS codes are evaluated in different case of interacting cracks problems. ASME Boiler and Pressure Vessel Code Section XI (ASME, 1998, 2004) and API 579 (ASME, 2007) defines that the multiple cracks are assumed to be independent until or unless the following conditions are satisfied. In the case of two parallel cracks in solid bodies, if distance between crack planes
2.3. Interacting cracks models for Fitness-for-Service
The solution for interacting surface or embedded cracks that based on FFS revision is limited in literature especially for interacting parallel edge cracks in finite body. Therefore, a review on available developed technique or models that related to FFS is presented in this section. The need of continues revision on FFS limitations based on ASME Boiler and Pressure Vessel Code Section XI and British Standard BS7910 started by the industrial failures in all major pressure vessels (Burdekin, 1982). The pressure vessels are designed and built to comply with ASME Boiler and Pressure Vessel Code Section XI and British Standard BS7910 codes but the failure occurrences are significantly high. Both codes can be expressed as
To investigate the problem, (Burdekin, 1982) studied the interaction between the collapse and fracture in pressure vessels using the approach that successfully applied to nuclear applications. The approach applied the LEFM and EPFM using COD and
Similarly, (O'donoghue et al., 1984) investigated the formation of elliptical cracks in aircraft and pressure vessel attachment lugs and identified the formation is due to stress risers and cracks interaction. Two equal coplanar surface cracks under Mode I loading are modeled using the proposed finite element alternating method (FEAM) in finite solid and the FE analysis results are compared to ASME Boiler and Pressure Vessel Code procedure. The interaction effects are defined by proposed magnification factor (normalized SIF) and the magnification factors seem to increase due to the increase interaction of two cracks and the depth of cracks. The Section XI of ASME Boiler and Pressure Vessel Code recommend that two interacting surface flaws in a pressure vessel should be modeled by a single elliptical crack that covers both flaws. It can be seen that SIF for single crack as proposed by FFS code are generally larger than those due to two interacting cracks as proposed by (O'donoghue et al., 1984). This trend of magnification factor shows that the ASME Boiler and Pressure Vessel Code in Section XI procedure will tend to underestimate the design life of multiple flaws structures. The ASME pressure vessel codes (ASME, 1998) and British Standard PD6495 (BSI, 1991) do not quantify the interaction between cracks especially in two close proximity cracks. At sufficiently close distance, the interaction may cause the increase of SIF. The exclusion of crack interaction may result with unrealistic SIF. Therefore, with the concern on the above standard guideline, (Leek & Howard, 1994) presents an empirical method to approximate the interaction factor of two coplanar surface cracks under tension and bending loading. The approximation approach resulted with good agreement with FE analysis using developed BERSAFE program, (Murakami & Nasser, 1982) and (J. C. Newman & Raju, 1981) within ± 5% discrepancy.
Based on the (ASME, 2004) and (BSI, 1991) design code that expressed by Eq. (1), (Moussa et al., 1999) used FEM to analyze interaction of two identical parallel non-coplanar surface cracks subjected to remote tension and pure bending loads. The interaction factor as a function of stress shielding to cause overlapping in distance is studied using three dimensional linear finite element analyses. The formation of stress relaxation state is introduced near crack front, as a form of shielding effect at sufficient overlapping.
where and are the SIFs with and without the influence of interaction, respectively. As conclusion, the interaction effect appears to diminish as the value of
The existing (ASME, 1998; JSME, 2000) FFS combination rules provided no prescription for the interference between multiple cracks for corrosion fatigue. Therefore, (Kamaya, 2003) developed simulation model to extent the condition of coalescence rules in (JSME, 2000) for crack growth process using body force method (BFM). BFM is used to investigate the multiple cracks growth in stress corrosion cracking. Based on JSME code and the SIF value of coalescence behavior from experiments, the new SIF formulation is developed using BFM where focus is given to the interaction between cracks under various relative position and size. The crack propagation direction can be written as
where the sign in Eq. (5) positive in the case of and negative in the case of . When the crack are close and overlapped, the crack interaction intensity between cracks is almost equivalent to single coalesced crack. The change of inner crack tips direction also found with little influence on the crack growth behavior. The relative crack length and position influenced the crack interaction intensity.
The combination rule in ASME Code is found to provide the relative large overestimation of the actual crack growth since the complex growth phenomena under interaction are summarized in simple combination rules. In order to reduce the conservativeness in existing code, (Kamaya, 2008b) proposed alternative assessment procedures based on the size of area and fatigue crack growth. Experimental analysis and testing is conducted using stainless steel specimens (A-H0S5 and B-H0S5) subjected to cyclic tensile loading. FE analysis is carried out to simulate the crack growth during coalescence. In the simulation, the automatic meshing was generated by command language in PATRAN and the SIF is derived from energy release rate obtained from virtual crack extension integral method using ABAQUS. The normalized SIF of Mode I, is expresses as
where denotes the applied tensile stress and the
where and are the material constant, denotes the Mode I SIF of the
In conclusion, the creep crack interaction represented by
Most recent, (Kamaya et al., 2010) used S-version finite element method to determine the SIF changes due to the interaction of stress field which caused variation in crack growth rate and cracks shape. The root of interaction problems is referred to (JSME, 2000, 2008) and (ASME, 2004, 2007) for the case of interacting dissimilar crack sizes. However, the effect of difference crack size or relative size effect is not taken into account in the aforementioned code. The results have shown that smaller cracks stopped growing when the difference in size of interaction was large enough. It means, the interaction effect on the fatigue life of the larger cracks was negligibly small. Moreover, the offset distance and the relative size were important parameter for interaction evaluation especially when the and the condition of crack spacing and cracks ratio must be considered most. In present study, the focus is given to determine the stage of crack interaction intensity is equal to single crack in a state of crack interaction limit (CIL) and unification (CUL) using finite element method.
3. Finite element analysis
3.1. Finite element analysis
The stress in the neighborhood of a crack tip in homogenous isotropic material exist in a form of square-root singular and there have been many special elements or singularity function based approach were described in details in (Banks-Sills, 1991). The square root singular stresses in the neighborhood can be modeled by quarter-point, square and collapsed, triangular elements for two dimensional problems, and by brick and collapsed, prismatic elements in three dimensions. Quarter-points square have been found to produce the most excellent results (Banks-Sills, 2010). The stiffness matrix of the element is evaluated using two-dimensional integral based on Gaussian quadrature approach. The plate is constructed with a consideration of singular element and assigned to both crack tips
3.1.1. Singularity stress field
The studies are conducted in a pure Mode I loading condition with specified material, Alloy 7475 T7351 solid plate in constant thickness, homogenous isotropic continuum material, linear elastic behavior, small strain and displacements, and crack surface are smooth. According to Westergaard method for single crack, Mode I and Mode II SIF can be expressed as:
where is nominal stress, is shear stress,
Consider two multiple edge crack of length and which occupies the segment of 0.05 ≤
According to Eq. (9), the shape correction factor can be converted to new elastic interaction factor
where and denotes to elastic interaction factor for Mode I and II fracture, respectively.
The SIF for Mode I and Mode II is determined using Displacement Extrapolation Method (DEM) by written APDL macro code in ANSYS (Madenci & Guven, 2006), and expressed as
4. Findings and discussion
Two parallel edge cracks interaction will mainly referred to shielding effect rather than amplification effect. The crack interaction is proportional to the magnitude of elastic interaction factor . The crack interaction will only exist at
and analytical single edge crack SIF reference by (Brown & Strawley, 1966),
4.1. Crack interaction factor comparison with analytical data
The mode I fracture of the elastic interaction factors for crack interval ratio and are shown in Fig. 3-6. Overall, it can be seen that the interaction factor varies with the different values where the crack interaction factor increases as the increases and vice versa. The point of intersection also observed occurred for all the values. For example, the plot of against at are illustrated in Fig. 3.The prediction line is compared with the predicted result of single edge crack . A general good agreement can be observed with a minimum difference 0.6% at and maximum difference 5.39 % difference. In comparison, the present has demonstrated more accurate prediction compared with results. For example, in reference to, at , the present prediction is in difference of 0.85 % and 0.4%, while is at 2.15% difference. In terms of the CIL point, the closer the crack interaction to of single crack, a more accurate CIL prediction can be achieved. It is noted that the analytical expression was formulated using the numerical results of
Theoretically, the study of intersection point is most significant in identification of crack interaction limit (CIL) and crack unification limit (CUL). The intersection point of two cracks with single crack justifies the realization of CIL at higher and CUL at lower . The CIL and CUL also differ with different . From Fig. 3, the identified CUL is at and CIL approximately at .
Another significant improvement of present is the moving intersection point as decreases for every , as shown in Fig. 3-6. From Fig. 4, the moving intersection point can be noticed moves from to . The moving intersection point exhibits similar prediction trend of . The intersection point also can be denoted as the crack unification limit (CUL) point, which indicates the starting point of strong interaction region start approximately at .
The intersection point is also observed to move from for , for , for and for , as shown in Fig. 4-6. It means that the CUL is not in a fix limit, it exist in dynamic condition which depends on crack interval ratio . Conversely, the prediction model overruled the FFS codes because it does not lead to a single independent or combined crack because of not having any intersection point. The intersection point could not be defined by prediction model.
It also can be seen that prediction is unable to display the unification of crack interaction factor, which defined equivalent to of single crack. In this case, the prediction is expected to encounter some numerical errors since at lower . In analysis, the ratio of crack length and width also define the critical stress field, if the path independent radius of
Based on the FFS codes, the multiple cracks are assumed to be independent as single cracks or combined cracks, until or unless certain conditions are satisfied. The intersection point that lies in the present prediction trend curve, which intersects with the single crack prediction, shows good agreement with the outlined FFS codes. It is seen that at range of , the value is about to level at 1.072 -1.085. The small changes in these range indicate that shielding effect is very small and promote the unification in interaction at the point of . The smaller the , the faster unification process starts.
4.2. Mode II fracture behavior
Fig. 7 depicts the trend of and against for . It can be seen that the increase in results in an increase of and a decrease of
values. In strong interaction region , the values of increased rapidly for higher crack-to-width ratio and before grew slowly as the value of decreases to . Meanwhile, the values of declined significantly at higher crack-to-width ratio and before decreased slightly as the value of decreases to . For both crack interaction phase, the value of is always much higher than . In weak interaction region , it can be seen that the values of increased slightly before growing slowly and then maintaining at the same level to steady state at . At the same region, the value of declined moderately before decreased slightly and remain stable at the level of . It means that mode II SIF is less influenced by damage shielding effect than mode I SIF. It also defined that the crack opening is more affected by damage shielding effect than the crack sliding. This has been clearly indicated in Fig. 7 (a)-(f) and Fig. 8(a)-(d).
From these figures, it also observed that the different between mode II SIF and mode I SIF is reduced as the decreases. In the context of crack interaction limit (CIL) based on and , by considering the convergence level as the indicator of CIL. It can be seen that the degree and speed of CIL achievement not only depends heavily on the increased of, the reduction of from also provides significant impact on CIL determination.
Fig. 8 shows the variation of and for . It can be observed that at smallest , the value of and is almost hold at constant value and stabilize.
The identification of CIL in this condition is absent because the value of and are about the same value for all . This equalization condition may be referred to the identification of crack unification limit (CIL). Overall, it can be concluded that the higher ratio of and , the more the realization of CIL. Inversely, the lower ratio of and , the more indication to CUL can be realized.
The numerical solution based on displacement extrapolation method (DEM) has proved to be more consistent in SIF prediction comparedd to for both crack tips. However, the DEM able to predict the SIF for Mode I and Mode II fracture behaviour. The FE results conclude that the interaction of two cracks is directly influence the reduction of SIF magnitude and at the crack tips. The parallel cracks have experienced decrease shielding effect as the cracks interval
Andersson B Blom A. F Falk U Wang G. S Koski K Siljander A et al 2009. Paper presented at the 25th ICAF Symposium.
ASME. ( 1998). ASME Boiler and Pressure Vessel Code, Section XI. New York, USA.
ASME. ( 2004). ASME Boiler and Pressure Vessel Code, Section XI. New York, USA.
ASME 2007 579 1FFS-1 Fitness-for-service, Section 9, New York, USA.
Banks-sills L 1991Application of the Finite Element Method to Linear Elastic Fracture Mechanics. Appl. Mech. Rev, 44 447 461
Banks-sills L 2010 Update: Application of the Finite Element Method to Linear Elastic Fracture MechanicsAppl. Mech. Rev, 63 1 17
Barsoum R. S 1974 Application of Quadratic Isoparametric Finite Elements in Linear Fracture Mechanics 10 603 605
Barsoum R. S 1975Further application of quadratic isoparametric finite element to linear fracture mechanics of plate bending and general rules. International Journal of Fracture, 11 167 169
Barsoum R. S 1976Application of Triangular Quarter-Point Elements as Crack Tip Elements of Power Law Hardening Material. International Journal of Fracture, 12 463 466
Brown W. F Strawley J. E 1966ASTM STP 410.
BSI 1991British Standard Institute, PD 6493, Section 8. .
BSI 1997British Standard Institute, BS7910, Section 8. .
BSI 2005British Standard Institute, BS7910. .
Burdekin F. M 1982 The role of fracture mechanics in the safety analysis of pressure vessels(4), 197 EOF 208 EOF
Chandrupatla T. R Belegundu A. D 2002(3rd ed.): Prentice Hall.
C. ( Chang J. I Lin C 2006 A study of storage tank accidents 19 51 59
Chen Y. Z Liu H. Y 1988Multiple cracks in pressurized hollow cyclinder. Theoritical and Applied Fracture Mechanics, 10 213 218
Garwood S. J 2001Investigation of the MV Kurdistan casuality. (1), 3-24.
Gorbatikh L Kachanov M 2000 A simple technique for constructing the full stress and displacement fields in elastic plates with multiple cracks 66 51 63
Henshell R. D Shaw K. G 1975 Crack tip finite elements are unnecessaryInt J Numer Engng, 9 495 507
Hu W Liu Q Barter S 2009. Paper presented at the 25th ICAF Symposium.
Ikeda T Nagai M Yamanaga K Miyazaki N 2006 Stress intensity factor analyses of interface cracks between dissimilar anisotropic materials using the finite element method 73 2067 2079
Isida M 1973 Analysis of stress intensity factors for the tension of a centrally cracked strip with stiffened edges 5 647 665
Jeong D. Y Brewer J. C 1995 On the linkup of multiple cracks 233 EOF 238 EOF
Jones R Peng D Pitt S 2002 Assessment of multiple flat elliptical cracks with interactionsTheoretical and Applied Fracture Mechanics, 38 281 291ssss.
JSME 2000JSME Fitness-for-Service Code S NA 1 2000
JSME 2008JSME Fitness-for-Service Code S NA 1 2008
Kamaya M 2003 A crack growth evaluation method for interacting multiple cracks(1), 15 EOF 23 EOF
Kamaya M 2008a Growth evaluation of multiple interacting surface cracks. Part II: Growth evaluation of parallel cracks 75 1350 1366
Kamaya M 2008b Growth evaluation of multiple interacting surface cracks.Part I: Experiments and simulation of coalesced crack. 75 1336 1349
Kamaya M Miyokawa E Kikuchi M 2010 Growth prediction of two interacting surface cracks of dissimilar sizes 77 3120 3131
Kirkhope K. J Bell R Kirkhope J 1991 Stress intensity factors for single and multiple semi-elliptical surface cracks in pressurized thick-walled cylindersInternational Journal of Pressure Vessel and Piping, 47 247 257
Kobayashi H Kashima K 2000 Overview of JSME flaw evaluation code for nuclear power plantsInternational Journal of Pressure Vessels and Piping, 77 937 944
Lakes R. S Nakamura S Behiri J. C Bonfield W 1990 Fracture mechanics of bone with short cracks.(10), 967 EOF 75 EOF
Lam K. Y Phua S. P 1991 Multiple crack interaction and its effect on stress intensity factor 585 EOF 592 EOF
Leek T. H Howard I. C 1994 Estimating the elastic interaction factor of two coplanar surface cracks under Mode I load.International Journal of Pressure Vessels and Piping, 60 307 321
Leek T. H Howard I. C 1996 An examination of methods of assessing interacting surface cracks by comparison with experimental dataInternational Journal of Pressure Vessels and Piping, 68 181 201
Lewis P. R Weidmann G. W 2001Catastropic failure of a polypropylene tank Part I: primary investigation. (4), 197-214.
Madenci E Guven I 2006(1 ed.): Springer Science-Business.
Matake T Imai Y 1977Pop-in behaviour induced by interaction of cracks. Engineering Fracture Mechanics, 9 17 24
Meizoso A. M Esnaola J. M. M Perez M. F 1995Interaction effect of multiple crack growth on fatigue. Theoretical and Applied Fracture Mechanics, 23 219 233
and accurate method for computing stress intensity factors of collinear interacting cracks. . Milwater H. R 2010 A Simple
Mischinski S Mural A 2011 Finite Element Modeling of Microcrack Growth in Cortical Bone 78 1 9
Moussa W. A Bell R Tan C. L 1999 The interaction of two parallel non-coplanar identical surface cracks under tension and bendingInternational Journal of Pressure Vessels and Piping, 76 135 145
Murakami Y 1976 A simple procedure for the accurate determination of stress intensity factors by finite element method 8 643 655
Murakami Y Nasser S. N 1982 Interacting dissimilar semi-elliptical surface flaws under tension and bending 373 EOF 386 EOF
Newman J. A Baughman J. M Wallace T. A 2010 Investigation of cracks found in helicopter longerons 17 416 430
Newman J. C Raju I. S 1981 An empirical stress intensity factor equation for the surface cracks. Engineering Fracture Mechanics, 15 185 192
S. N. ( O Donoghue P. E Nishioka T Atluri 1984 Multiple surface cracks in pressure vessel. 545 EOF 560 EOF
Pant M Singh I. V Mishra B. K 2011 A numerical study of crack interactions under thermo-mechanical load using EFGM 403 EOF 413 EOF
Park C. H Bobet A 2010Crack initiation, propagation and coalescence from frictional flaws in uniaxial compression. Engineering Fracture Mechanics, 77 2727 2748
Parker A. P 1999 Stability of arrays of multiple edge cracks 62 577 591
Pitt S Jones R Atluri S. N 1999 Further studies into interacting 3D cracksComputers and Structures, 70 583 597
- 54. R6. (2006). Nuclear Electric : Assessment of the integrity of structures containing defects, Revision 4. Gloucester, British Energy Generation Ltd.
Ratwani M Gupta G. D 1974Interaction between parallel cracks in layered composites. International Journal of Solids and Structures, 10 701 708
Rutti T. F Wentzel E. J 1997Investigation of failed actuator piston rods. (2), 91-98.
Saha T. K Ganguly S 2005Interaction of penny-shaped cracks with an eliptic crack under shear loading. International Journal of Fracture, 131 267 287
Sankar R Lesser A. J 2006 Generic Overlapping Cracks in Polymers: Modeling of InteractionInternational Journal of Fracture, 142 277 287
Sekhtar A. S 2008Multiple cracks effects and identification. Mechanical Systems and Signal Processing, 22 845 878
Shields E. B Srivatsan T. S Padovan J 1 EOF 26 EOF
Shivakumar K. N Raju I. S 1992 An equivalent domain integral method for three-dimensional mixed-mode fracture problemsEngineering Fracture Mechanics, 42 935 959
Ural A Zioupos P Buchanan D Vashishth D 2011 The effect of strain rate on fracture toughness of human cortical bone: A finite element study.
Weidmann G. W Lewis P. R 2001Catastropic failure of a polypropylene tank Part II: comparison of the DVS 2205 code of practice and the design of the failed tank. (4), 215-232.
S. T. ( Xuan F Z Si J Tu 2009 Evaluation of C* integral for interacting cracks in plates under tension 76 2192 2201
Yang Y. H 2009 Multiple parallel symmetric mode III cracks in a functionally graded material plane 819 EOF 830 EOF
Z. D Jiang A Zeghloul G Bezine J Petit 1990 Stress intensity factor of parallel cracks in a finite width sheet. 1073 EOF 1079 EOF
Z. D Jiang J Petit G Bezine 1990 Fatigue propagation of two parallel cracks 1139 EOF 1144 EOF